|Year : 2021 | Volume
| Issue : 2 | Page : 186-191
Effect of freshly placed core buildup composites on setting of silicon impression materials
Mohammad A Al-Rabab'ah1, Muhanad M Hatamleh2, Sandra Al-Tarawneh3, Ahmad El-Ma'aita1, Ibrahim Abu Tahun1, Issam S Jalham4
1 Department of Conservative Dentistry, University of Jordan, Amman, Jordan
2 Department of Dental Technology, Luminus Technical University, Amman, Jordan
3 Department of Removable Prosthodontics, The University of Jordan, Amman, Jordan
4 Department of Industrial Engineering, The University of Jordan, Amman, Jordan
|Date of Submission||07-Dec-2020|
|Date of Decision||22-Feb-2021|
|Date of Acceptance||11-Mar-2021|
|Date of Web Publication||28-Apr-2021|
Mohammad A Al-Rabab'ah
Department of Conservative Dentistry, University of Jordan, Amman 11942
Source of Support: None, Conflict of Interest: None
Aim: The aim is to study the effect of freshly placed composite build-ups on setting of additional silicone impression materials.
Settings and Design: In vitro - experimental study.
Materials and Methods: Three composite materials; Build-It™ F. R™, Filtek™ Bulk Fill flow and Filtek™ Z350 and three light-bodied additional silicone impression materials; Elite HD+, Aquasil LV Ultra and Express™ were used. Cylindrical-shaped specimens were made of each material (diameter 15 mm and height 10 mm). The silicone specimens were brought into contact with the composite specimens, which were either freshly cured (9 groups, n = 90) or cured and then stored in normal saline for 1 week (9 groups, n = 90). Shore A hardness (SAH) scores of silicone surfaces were recorded following the ASTM D2240-5 standards for shore A Durometer testing. Six measurements were made per each silicone surface and medians were calculated. Kruskal–Wallis and Mann–Whitney tests (SPSS v20) were used to check statistical significant differences between all groups and paired comparisons, respectively (P < 0.05).
Statistical Analysis Used: Kruskal-Wallis and Mann-Whitney tests.
Results: The SAH scores of additional silicones in direct contact with freshly placed composites were significantly less than SAH scores of additional silicones in direct contact with composites specimens aged for 1 week in 7 out of 9 combinations (P < 0.05). Only when Express™ and Elite HD+ were applied over freshly placed Filtek™ Bulk Fill flow, the SAH scores difference was not statistically significant to SAH scores of matching combinations applied after 1 week of composite storage.
Conclusions: Freshly placed composite might affect setting of additional silicone impression materials. Dentists should carefully assess final impression on areas of prepared teeth that have received composite fillings recently.
Keywords: Additional silicon, composites, core build-up, shore A hardness
|How to cite this article:|
Al-Rabab'ah MA, Hatamleh MM, Al-Tarawneh S, El-Ma'aita A, Tahun IA, Jalham IS. Effect of freshly placed core buildup composites on setting of silicon impression materials. J Indian Prosthodont Soc 2021;21:186-91
|How to cite this URL:|
Al-Rabab'ah MA, Hatamleh MM, Al-Tarawneh S, El-Ma'aita A, Tahun IA, Jalham IS. Effect of freshly placed core buildup composites on setting of silicon impression materials. J Indian Prosthodont Soc [serial online] 2021 [cited 2021 Aug 3];21:186-91. Available from: https://www.j-ips.org/text.asp?2021/21/2/186/315070
| Introduction|| |
Resin composites are the preferred choice for direct fillings and core build-ups in vital and root canal treated teeth particularly when metal-free indirect restorations are planned., Resin composites and their flowable and bulk fill variants might be used to optimize the preparation design for an endocrown, seal endodontic access, fill small gaps or create an entire core build up with or without posts.
To shorten temporization period and provide better long-term seal final impression is usually made at the same visit of placing direct filling over endodontically treated teeth. The ability to take final impression directly after fillings/core buildup will reduce clinical time and any negative effect of provisional restorations on final impression. A highly accurate impression of prepared teeth is crucial to provide a successful indirect restoration. Many clinical steps affect setting of rubber impression materials. Freshly placed composites will have layer of unreactive resin monomer, which might interfere with the polymerization of the impression materials.
Currently, only additional silicones and polyether impression materials can attain the rigors requirements to qualify for final impression of crowns, fixed partial dentures, and implant work. During the stage of final impression, dimensional accuracy and stability are important to achieve to produce a true replica of the prepared teeth, implants and vicinity. Although digital scanners can achieve “virtual” unlimited stability to the details of prepared teeth/implant vicinity their use is still limited by their expensive capital investment to any dental surgery. Digital dentistry also has different platforms that are sometimes not easily synchronized with the daily work of a dental practice and would require an elaborative learning curve that some dentists might find cumbersome. Intraoral scanners are used nowadays to capture details of prepared teeth and implants to construct restorations. The accuracy of scanners has been found to match that of additional silicone impression materials., Some studies have shown that intraoral scanners are less accurate when capturing details of full arch reconstructions or postpreparations., Scanners also are less suited for capturing subgingival details when preparations of teeth are cervical to the gingival margin.
Few clinical steps might affect the setting of additional silicone impression materials. Latex gloves have been implicated in delaying or completely inhibiting setting additional silicone impression materials. Vinyl Gloves showed no interaction with the setting of silicone impression materials. Hemostatic agents and retraction cords and retraction pastes were also tested for possible interactions., Interim resin materials and cements might also affect polymerization of elastomeric impression materials. Hardness of silicone materials might also change after setting when those materials are disinfected.,,
The aim of this study was to investigate if freshly placed composite might affect setting of additional silicone impression materials through testing of Shore A Hardness (SAH) test and to compare those specimens with additional silicone specimens made in contact with composites specimens that were stored for 1 week. Our null hypothesis indicates that freshly placed composite will not affect SHA of additional silicone materials.
| Materials and Methods|| |
The study was approved by institutional review board. Transparent polylactic acid molds were 3D printed according to standard test method as set in ASTM D2240-5 for shore A Durometer testing. For Silicone molds cylinders were made (diameter 15 mm and 10 mm height) with 2 mm rim leaving 13 mm of hollow width to be filled with the additional silicone during testing [Figure 1]. Composite specimens were made using cylindrical molds of similar width but only 3 mm height [Figure 2]. Thirty silicone specimens were used as control without contact with composite (10 for each group). Composite materials used in this experiment are listed in [Table 1]. All composite materials were applied to their respective molds and covered by glass slides before irradiated with LED (starlight pro, mectron, Carasco, Italy) for 40s each side. The light intensity was 800 mW/cm2. Additional silicone materials were all light bodied variants and are listed in [Table 2]. All impression specimens were mixed using compatible Automixing cartridge and mixing tips and brought in direct contact with composite molds using digital pressure through firm application of glass slide for 8 min. A 180 specimens were in direct contact [Figure 3] with either freshly placed and cured composites (n = 90) or composites specimens that were stored in normal saline for 7 days (n = 90). [Table 3] lists all groups tested in this study.
|Figure 3: Silicone specimen brought in direct contact with aged composite|
Click here to view
Shore A scores were recorded after 10 min of initial setting by a laboratory technician who was blinded to the nature of test groups. Type PG, W-Testor Otto, Wolpert-Werke (Ludwigshafen, Germany) was used to record the Shore A scores. 6 readings were made per each side of the silicone and medians of each side were calculated. Contacting sides with composites were plotted against control and rear side. Shore A scores of freshly placed specimens were compared with those of 1 week specimens.
Statistical analysis was carried out using SPSS version 20 (IBM, Armonk, NY, USA). Kruskal–Wallis test was used to check for statistical significant difference. Mann–Whitney tests were used to compare individual combinations (same day vs. 1 week).
| Results|| |
Control groups SAH medians were 47 (0.6) for Express, 60 (1.5) for Aquasil and 53 (0.4) for Elite. [Table 4] shows the decrease in percentage of SAH for test specimens for sides in direct contact with composite specimens when compared to the rear side of each specimen. Rear sides scores of SAH did not have any significant difference to those of control groups There was a general tendency for decrease in SAH scores in the groups where setting silicone was brought into contact with freshly cured composites. When aged composite specimens for 1 week were used SAH scores of additional silicones there were no significant difference to the controls. Groups 1–9 were in direct contact with freshly placed composites while groups 10–18 were placed over composite specimens made 1 week before. [Table 5] shows median and standard deviation of SAH for each group.
|Table 4: Percentage of reduction in shore A hardness of surfaces contacting composite specimens compared to rear side|
Click here to view
|Table 5: Shore A hardness scores medians (standard deviation) for tested groups|
Click here to view
Nine runs of Mann–Whitney test for the combination of groups of the same silicone and composite materials tested at same day and 1 week respectively revealed that null hypothesis was rejected in seven combinations out of 9 where SAH scores of silicone materials in direct contact with freshly placed composites were significantly lower than their counterparts made in direct contact with composite aged for 1 week. [Table 6] shows the results of Mann–Whitney tests.
| Discussion|| |
Additional silicones are widely used as final impression material when capturing details of teeth, implants, and also edentulous jaws. Due to their high dimensional accuracy and stability, they can be considered as gold standards to which new techniques or materials are often compared. Their setting reaction involves mainly polymerization by chain lengthening and cross linking through additional reaction of Vinyl silicone group. The catalyst used is mainly platinum-containing compound. No by-products are produced apart from hydrogen gas (H2), which is produced in some additional silicone variants by secondary reaction. Setting of additional silicone is sensitive to moisture. Water can have detrimental effect on setting of those impression materials.
SAH test was used to study the effect of different factors on setting reaction of additional silicones. Changes in SAH will also have impact on Young's modulus of the impression material and any decrease in SAH might affect setting and elastic recovery of impression material leading to inaccurate impression or and low tear resistance. In this study, the use of SAH provided a reliable quantitative comparison of setting of additional silicone materials. Previous studies had employed qualitative evaluation of the setting of impression materials.,,,,
The degree of conversion of dental composites is well <100% and unreactive monomer will still be present in set composite.,, Immediate sealing of dentin of prepared teeth has been shown to adversely affect the setting of silicone and polyether impression materials alike., Few maneuvers were attempted to alleviate this negative effect of an acclaimed superior technique. Applying glycerin gel or alcohol and further curing the bonding agent or flowable composite might reduce the oxygen-inhibiting layer (OIL). Studies suggested that the unreactive monomer in the OIL was responsible for the incomplete setting of the silicone material but mechanism is still unknown. It has been postulated that the acidity of OIL will affect the setting reaction of self-curing polymers., The OIL layer is basically a photointiator-deprived uncured resin. OIL was found to promote better bonding in few studies while other studies have shown a negative impact of OIL on bonding. The nature of the effect of OIL in bonding might be dependent on the adhesive molecule., The OIL was found to be thicker with unfilled resin when compared to filled resins. Normally OIL layer can be made thinner by air-blocking (application of glycerine gel) or with pumicing. It can also be reduced using water spraying or application of ethanol-soaked cotton pledget for about 20 s.
In the present study, composite specimens were covered by glass slide and irradiated with the light cure before additional silicone impression materials applied. Even with the use of air blocking, OIL might still be present but is normally thinner. Water spraying is thought to only minimize the OIL. It can be postulated that water storage of composite specimens removed the OIL and thus SAH of impression materials specimens brought into contact with 1-week water aged composite were not significantly different than control groups. When composite specimens were only air-aged bond interlayer strengths started to deteriorate only after 14 days.
Taking impression directly after placing composite fillings and core build-ups will reduce temporization time and aging of the composite material. Bonding strengths of adhesive cements to composite aged for more than 14 days was inferior when compared to bonding strengths for composites aged for a week or less. Deferring the impression stage to 1 week later will lessen the effect of OIL and free radicals on the setting reaction of impression materials. If clinician prefers to take final impression at the same visit of core build-ups any composite restoration should either be sprayed with water or soaked with alcohol or hydrogen peroxide. Dry preparation should be avoided. Clinician should always critically inspect impressions taken when composite fillings/build-ups are part of the prepared tooth/teeth. Special attention should be made to ensure complete setting of silicone impression materials and this should preferably be done under magnification. Further research is needed to provide maneuvers to remove OIL layer when attempting to take impression at the same visit while not affecting bond strength to resin adhesive luting cements later.
| Conclusions|| |
Within the limitations of this study, it can be concluded that freshly placed composite might affect setting of additional silicon impression materials. Water spraying or application of alcohol soaked cotton pellet is advised. Dentists should carefully assess final impression on areas of prepared teeth that have received composite fillings recently.
Financial support and sponsorship
Conflicts of interest
There are no conflicts of interest.
| References|| |
Carvalho AO, Bruzi G, Anderson RE, Maia HP, Giannini M, Magne P. Influence of adhesive core buildup designs on the resistance of endodontically treated molars restored with lithium disilicate CAD/CAM crowns. Oper Dent 2016;41:76-82.
Magne P, Goldberg J, Edelhoff D, Güth JF. Composite resin core buildups with and without post for the restoration of endodontically treated molars without ferrule. Oper Dent 2016;41:64-75.
Al-Sayeda H, Al-Resayesa S, Jamjooma F, Al-Sowyghb Z. The effect of various core build-up materials on the polymerization of elastomeric impression materials.King Saud J Dent Sci 2013;4:71-5.
Marghalani A, Weber HP, Finkelman M, Kudara Y, El Rafie K, Papaspyridakos P. Digital versus conventional implant impressions for partially edentulous arches: An evaluation of accuracy. J Prosthet Dent 2018;119:574-9.
Polyzois G, Lyons K. Monitoring Shore A hardness of silicone facial elastomers: The effect of natural aging and silicone type after 1 year. J Craniofac Surg 2014;25:1217-21.
Pinto A, Arcuri L, Carosi P, Nardi R, Libonati A, Ottria L, et al
. In vitro
evaluation of the post-space depth reading with an intraoral scanner (IOS) compared to a traditional silicon impression. Oral Implantol (Rome) 2017;10:360-8.
Patzelt SB, Bishti S, Stampf S, Att W. Accuracy of computer-aided design/computer-aided manufacturing-generated dental casts based on intraoral scanner data. J Am Dent Assoc 2014;145:1133-40.
Nedelcu R, Olsson P, Nyström I, Thor A. Finish line distinctness and accuracy in 7 intraoral scanners versus conventional impression: An in vitro
descriptive comparison. BMC Oral Health 2018;18:27.
Ravikumar CM, Sangur R. Effect of five brands of latex gloves on the setting time of polyvinyl siloxane putty impression materials. Indian J Dent Res 2012;23:209-12. [Full text]
Machado CE, Guedes CG. Effects of sulfur-based hemostatic agents and gingival retraction cords handled with latex gloves on the polymerization of polyvinyl siloxane impression materials. J Appl Oral Sci 2011;19:628-33.
Abduljabbar TS, Al Amri MD, Al Rifaiy MQ, Al-Sowygh ZH, Vohra FA, Balous MA, et al
. Effects of gingival retraction paste and subsequent cleaning with hydrogen peroxide on the polymerization of three elastomeric impression materials: An In vitro
study. J Prosthodont 2019;28:709-14.
Al-Sowygh ZH. The effect of various interim fixed prosthodontic materials on the polymerization of elastomeric impression materials. J Prosthet Dent 2014;112:176-81.
Eleni PN, Krokida MK, Polyzois GL, Gettleman L. Effect of different disinfecting procedures on the hardness and color stability of two maxillofacial elastomers over time. J Appl Oral Sci 2013;21:278-83.
Khinnavar PK, Kumar BH, Nandeeshwar DB. An in vitro
study to evaluate the effect on dimensional changes of elastomers during cold sterilization. J Indian Prosthodont Soc 2015;15:131-7.
] [Full text]
Badrian H, Davoudi A, Molazem M, Zare MH. The effect of spraying different disinfectants on condensational silicone impressions; an in vitro
study. J Indian Prosthodont Soc 2015;15:263-7.
] [Full text]
Hyde TP, Craddock HL, Gray JC, Pavitt SH, Hulme C, Godfrey M, et al
. A randomised controlled trial of complete denture impression materials. J Dent 2014;42:895-901.
McCabe JF, Walls AW. Applied Dental Materials. 9th
ed. Hoboken, New Jersey, USA: Blackwell; 2008.
Hosseinpour D, Berg JC. The dynamic interaction of water with four dental impression materials during cure. J Prosthodont 2009;18:292-300.
Meththananda IM, Parker S, Patel MP, Braden M. The relationship between Shore hardness of elastomeric dental materials and Young's modulus. Dent Mater 2009;25:956-9.
Moon MG, Jarrett TA, Morlen RA, Fallo GJ. The effect of various base/core materials on the setting of a polyvinyl siloxane impression material. J Prosthet Dent 1996;76:608-12.
Magne P, Nielsen B. Interactions between impression materials and immediate dentin sealing. J Prosthet Dent 2009;102:298-305.
Ghiggi PC, Steiger AK, Marcondes ML, Mota EG, Burnett LH Júnior, Spohr AM. Does immediate dentin sealing influence the polymerization of impression materials? Eur J Dent 2014;8:366-72. [Full text]
Ferracane JL, Hilton TJ, Stansbury JW, Watts DC, Silikas N, Ilie N, et al
. Academy of Dental Materials guidance-Resin composites: Part II-Technique sensitivity (handling, polymerization, dimensional changes). Dent Mater 2017;33:1171-91.
Bergmann P, Noack MJ, Roulet JF. Marginal adaptation with glass-ceramic inlays adhesively luted with glycerine gel. Quintessence Int 1991;22:739-44.
Suh BI. Oxygen-inhibited layer in adhesion dentistry. J Esthet Restor Dent 2004;16:316-23.
Sanares AM, Itthagarun A, King NM, Tay FR, Pashley DH. Adverse surface interactions between one-bottle light-cured adhesives and chemical-cured composites. Dent Mater 2001;17:542-56.
Tsujimoto A, Barkmeier WW, Takamizawa T, Latta MA, Miyazaki M. Influence of the oxygen-inhibited layer on bonding performance of dental adhesive systems: Surface free energy perspectives. J Adhes Dent 2016;18:51-8.
Dall'Oca S, Papacchini F, Goracci C, Cury AH, Suh BI, Tay FR, et al
. Effect of oxygen inhibition on composite repair strength over time. J Biomed Mater Res B Appl Biomater 2007;81:493-8.
Rueggeberg FA, Margeson DH. The effect of oxygen inhibition on an unfilled/filled composite system. J Dent Res 1990;69:1652-8.
Bijelic-Donova J, Garoushi S, Lassila LV, Vallittu PK. Oxygen inhibition layer of composite resins: Effects of layer thickness and surface layer treatment on the interlayer bond strength. Eur J Oral Sci 2015;123:53-60.
Ben-Amar A, Geiger S, Liberman R. Effect of water spray on lining materials and their adhesion to composite and dentin cavity walls. Dent Mater 1991;7:274-8.
[Figure 1], [Figure 2], [Figure 3]
[Table 1], [Table 2], [Table 3], [Table 4], [Table 5], [Table 6]